Self-assembly of gold nanoparticles to silver microspheres as highly efficient 3D SERS substrates
- Shouhui Chen†1, 2,
- Peng Huang†2,
- Zhihua Wang2,
- Zhe Wang2,
- Magdalena Swierczewska2,
- Gang Niu2,
- Daxiang Cui1Email author and
- Xiaoyuan Chen2Email author
© Chen et al.; licensee Springer. 2013
Received: 6 March 2013
Accepted: 17 March 2013
Published: 12 April 2013
Herein we report a simple, one-pot, surfactant-free synthesis of 3D Ag microspheres (AgMSs) in aqueous phase at room temperature. The 3D AgMSs act as supports to fix the gold nanoparticles (GNPs) in 3D space via the interaction between the carboxyl groups of GNPs and the Ag atoms of AgMSs. The ensemble of AgMSs@GNPs with high surface-enhanced Raman scattering (SERS) activity and sensitivity can be an ideal 3D substrate choice for practical SERS detection applications. The simple self-assembly strategy may be extended to other metallic materials with great potentials in SERS, catalysis, and photoelectronic devices.
KeywordsSelf-assembly Gold nanoparticles Silver microspheres SERS
Ensembles of inorganic nanoparticles, which display unique collective properties that are different from those of both the individual nanoparticles and bulk materials, are of much scientific and technological interest [1–5]. The ensembles have the following potential advantages: (1) to display new electronic, magnetic, and optical properties as a result of interactions between the excitons, magnetic moments, or surface plasmons of individual nanoparticles; (2) to improve the mechanical properties of composite materials; and (3) to allow multiple tasks to be performed simultaneously or in sequence. Typically, the self-assembly of noble-metal nanoparticles has attracted much attention because of their unique plasmon resonance and their tremendous applications in the area of optical waveguides , superlensing , photon detection , and surface-enhanced Raman scattering (SERS) [9–12]. Recently, the SERS effect based on noble-metal ensembles is of particular interest because of its extraordinary ability to detect a wide variety of chemical/biological species at extremely low concentrations even down to the single-molecule level .
Gold nanoparticles (GNPs) have been widely used as Raman active substrates because of their good biocompatibility and strong SERS enhancement [13–18]. However, it should be mentioned that the particles tend to aggregate during aging, which results in an unwanted reduction of the active surface area [19, 20]. To address this issue, the fixation of GNPs in one-dimensional (1D), 2D, or 3D spaces can avoid the aggregation of the particles as SERS substrates. Tsukruk et al. assembled GNPs onto 1D silver nanowires and 2D silver nanoplates to create bimetallic nanostructures as efficient single-nanoparticle Raman markers . Li et al. developed a 2D GNP monolayer film as SERS substrate by the self-assembly of nanoparticles at a liquid/liquid interface . Zhang et al. reported that GNPs dispersed on the grapheme oxide (GO, 2D) and reduced graphene oxide (RGO, 2D) supports exhibit excellent SERS and catalytic performance compared with the metal nanoparticles alone . Qian et al. prepared the self-assembled 3D-ordered GNP precursor composite (SiO2/GNPs) arrays as SERS nanoprobes . Choi et al. reported a highly ordered SERS-active surface that is provided by a 3D GNP array based on thermal evaporation of gold onto an indium tin oxide (ITO) surface through a nanoporous alumina mask . This SERS-active surface was applied to analyze the intracellular state. Therefore, the development of appropriate support materials to fix GNPs is very important in practical SERS detection applications.
Recently, 3D Ag microspheres (AgMSs), which contain special fine structure, large specific surface area, and micron-sized particles, have been applied as SERS substrates [19, 26]. For example, Zhao et al. prepared 3D AgMSs with nanotextured surface morphology by a simple, sonochemical, surfactant-free method. Due to their special structural features with nanoscale corrugations, the obtained 3D silver microstructures showed a structurally enhanced SERS performance . Zhang et al. developed hierarchical assemblies of silver nanostructures as highly sensitive SERS platforms by an acid-directed assembly method . Our group also used proteins  and microorganisms  as templates to synthesize AgMSs and hollow porous AgMSs, respectively. However, the controlled synthesis of AgMSs with clean rough surface is still a significant challenge.
Preparation of gold nanoparticles
Briefly, 50 mL (0.2 mg/mL) of chloroauric acid (Sigma-Aldrich) was heated to boiling point, and then 1.2 mL (10 mg/mL) of sodium citrate (Sigma-Aldrich) was added. Boiling lasted for 5 min until the solution became dark red in color. After cooling down to room temperature, 20 μL of GNPs was used for the analysis using transmission electron microscopy (TEM).
Zeta potential of the assemblies prepared at different molar ratios of Ag microspheres to gold nanoparticles
Typically, 2.5 mL of 5 mM AgNO3 aqueous solution was added to 95 mL of deionized (DI) water in a 150-mL beaker. Then, 2.5 mL of 5 mM l-AA (Sigma-Aldrich) was added into the above-mentioned solution under vigorous stirring at room temperature. The system was stirred vigorously under ambient conditions for 4 h. The color of the solution rapidly changed from colorless to gray. The resulting product was collected by centrifugation, washed three times with DI water and ethanol, and then dispersed in ethanol for further use.
Preparation of the assemblies of GNPs to AgMSs
AgMSs (10.8 mg) was dispersed in 0.9 mL of ethanol solution, then 100 μL of different concentrations of GNPs (0.4, 0.2, 0.1, 0.02, and 0.01 mg) were mixed with AgMSs solution under ultrasonic interaction, respectively. After 10 min, the resulting product was collected by centrifugation at 1,000 rpm for 5 min and washed twice with DI water and then dispersed in 1 mL DI H2O for further use.
Preparation of Raman samples
A total of 200 μL of GNPs to AgMSs (AgMSs@GNPs) was immersed in ethanol solutions containing 200 μL of 2-mercaptopyridine (2-Mpy) (10 to 7 M) under ultrasound for 10 min. After 2-Mpy molecules (Sigma-Aldrich) were adsorbed on the AgMSs@GNPs, the samples were washed twice with DI water and ethanol by centrifugation and finally dispersed in 10 μL ethanol. Then, an aliquot of 10 μL of 2-Mpy-loaded AgMSs@GNPs in ethanol solution was dropped onto a Si wafer. The dropped solution was spread evenly into a circle. After evaporation of ethanol under the dry N2, the sample was measured by a simple Raman instrument for six times. All of the experiments were carried out at room temperature.
The UV-visible spectra were recorded in a Shimadzu UV-2450 UV-visible spectrophotometer (Shimadzu Co. Ltd., Beijing, China) from 300 to 600 nm. DI water was used as the blank. SEM images were taken on a ZEISS-ULTRA 55 scanning electron microscope (Carl Zeiss AG, Oberkochen, Germany). For TEM, a drop of aqueous solution containing the samples was placed on the carbon-coated copper grids and dried under an infrared lamp for 30 min. The micrographs were obtained using a JEOL JEM-2010 transmission electron microscope (JEOL Ltd., Tokyo, Japan) operating at an accelerating voltage of 200 kV. Electron diffraction patterns were also recorded for the selected area. The surface charge of the samples was performed on NICOMP 380ZLS (Zeta potential/particle sizer; Agilent Technologies Inc., Santa Clara, CA, USA) system. SERS spectra of 2-Mpy-loaded AgMSs@GNPs were recorded by a simple Raman instrument (BWS415 B&W Tek Inc., Newark, DE, USA).
Results and discussion
In summary, we report a simple, one-pot, surfactant-free synthesis of 3D AgMSs in aqueous phase at room temperature. The 3D AgMSs act as supports to fix the GNPs in 3D space via the interaction between the carboxyl groups of GNPs and the Ag atoms of AgMSs. The ensemble of AgMSs@GNPs with high SERS activity and sensitivity can be an ideal 3D substrate choice for practical SERS detection applications. The simple self-assembly strategy may be extended to other metallic materials with great potentials in SERS, catalysis, photoelectronic devices, etc.
This work was supported in part by the Intramural Research Program (IRP), National Institute of Biomedical Imaging and Bioengineering (NIBIB), National Institutes of Health (NIH), the National Key Basic Research Program (973 Project) (2010CB933902 and 2011CB933100), National 863 Hi-tech Project (2007AA022004), Important National Science & Technology Specific Projects (2009ZX10004-311), National Natural Scientific Fund (nos. 81225010, 20771075, 20803040, and 81028009), New Century Excellent Talent of Ministry of Education of China (NCET-08-0350), and Shanghai Science and Technology Fund (10XD1406100).
- Nie ZH, Fava D, Kumacheva E, Zou S, Walker G, Rubinstein M: Self-assembly of metal–polymer analogues of amphiphilic triblock copolymers. Nat Mater 2007, 6: 609–614. 10.1038/nmat1954View Article
- Nie ZH, Petukhova A, Kumacheva E: Properties and emerging applications of self-assembled structures made from inorganic nanoparticles. Nat Nanotechnol 2010, 5: 15–25. 10.1038/nnano.2009.453View Article
- Nie ZH, Li W, Seo M, Xu SQ, Kumacheva E: Janus and ternary particles generated by microfluidic synthesis: design, synthesis, and self-assembly. J Am Chem Soc 2006, 128: 9408–9412. 10.1021/ja060882nView Article
- Xia YS, Nguyen TD, Yang M, Lee B, Santos A, Podsiadlo P, Tang ZY, Glotzer S, Kotov N: Self-assembly of self-limiting monodisperse supraparticles from polydisperse nanoparticles. Nat Nanotechnol 2011, 6: 580–587.View Article
- He D, Hu B, Yao QF, Wang K, Yu SH: Large-scale synthesis of flexible free-standing SERS substrates with high sensitivity: electrospun PVA nanofibers embedded with controlled alignment of silver nanoparticles. ACS Nano 2009, 3: 3993–4002. 10.1021/nn900812fView Article
- Maier SA, Kik PG, Atwater HA, Meltzer S, Harel E, Koel BE, Requicha AA: Local detection of electromagnetic energy transport below the diffraction limit in metal nanoparticle plasmon waveguides. Nat Mater 2003, 2: 229–232. 10.1038/nmat852View Article
- Fang N, Lee H, Sun C, Zhang X: Sub-diffraction-limited optical imaging with a silver superlens. Science 2005, 308: 534–537. 10.1126/science.1108759View Article
- Konstantatos G, Clifford J, Levina L, Sargent EH: Sensitive solution-processed visible-wavelength photodetectors. Nat Photonics 2007, 1: 531–534. 10.1038/nphoton.2007.147View Article
- Zhu ZN, Meng HF, Liu WJ, Liu XF, Gong JX, Qiu XH, Jiang L, Wang D, Tang ZY: Superstructures and SERS properties of gold nanocrystals with different shapes. Angew Chem Int Ed Engl 2011, 50: 1593–1596. 10.1002/anie.201005493View Article
- Lu G, Li H, Liusman C, Yin ZY, Wu SX, Zhang H: Surface enhanced Raman scattering of Ag or Au nanoparticle-decorated reduced graphene oxide for detection of aromatic molecules. Chem Sci 2011, 2: 1817–1821. 10.1039/c1sc00254fView Article
- Lu G, Li H, Wu SX, Chen P, Zhang H: High-density metallic nanogaps fabricated on solid substrates used for surface enhanced Raman scattering. Nanoscale 2011, 4: 860–863.View Article
- Braun G, Pavel I, Morrill AR, Seferos DS, Bazan GC, Reich NO, Moskovits M: Chemically Patterned microspheres for controlled nanoparticle assembly in the construction of SERS hot spots. J Am Chem Soc 2007, 129: 7760–7761. 10.1021/ja072533eView Article
- Emory SR, Haskins WE, Nie SM: Direct observation of size-dependent optical enhancement in single metal nanoparticles. J Am Chem Soc 1998, 120: 8009–8010. 10.1021/ja9815677View Article
- Krug JT, Wang GD, Emory SR, Nie SM: Efficient Raman enhancement and intermittent light emission observed in single gold nanocrystals. J Am Chem Soc 1999, 121: 9208–9214. 10.1021/ja992058nView Article
- Qian XM, Peng XH, Ansari D, Yin QG, Chen GZ, Shin DM, Yang L, Young A, Wang DM, Nie SM: In vivo tumor targeting and spectroscopic detection with surface-enhanced Raman nanoparticle tags. Nat Biotechnol 2008, 26: 83–90. 10.1038/nbt1377View Article
- Liu HN, Li S, Liu LS, Tian L, He NY: An integrated and sensitive detection platform for biosensing application based on Fe@Au magnetic nanoparticles as bead array carries. Biosens Bioelectron 2010, 26: 1442–1448. 10.1016/j.bios.2010.07.078View Article
- Huang P, Lin J, Li ZM, Hu HY, Wang K, Gao G, He R, Cui DX: A general strategy for metallic nanocrystals synthesis in organic medium. Chem Commun 2010, 46: 4800–4802. 10.1039/c0cc00307gView Article
- Li S, Liu H, Jia YY, Deng Y, Zhang LM, Lu ZX, He NY: A novel SNPs detection method based on gold magnetic nanoparticles array and single base extension. Theranostics 2012, 2: 967–975. 10.7150/thno.5032View Article
- Zhang MF, Zhao AW, Sun HH, Guo HY, Wang DP, Li D, Gan ZB, Tao WY: Rapid, large-scale, sonochemical synthesis of 3D nanotextured silver microflowers as highly efficient SERS substrates. J Mater Chem 2011, 21: 18817–18824. 10.1039/c1jm12831kView Article
- Zhang MF, Zhao AW, Guo HY, Wang DP, Gan ZB, Sun HH, Li D, Li M: Green synthesis of rosettelike silver nanocrystals with textured surface topography and highly efficient SERS performances. Cryst Eng Comm 2011, 13: 5709–5717. 10.1039/c1ce05105aView Article
- Gunawidjaja R, Kharlampieva E, Choi I, Tsukruk V: Bimetallic nanostructures as active Raman markers: gold-nanoparticle assembly on 1D and 2D silver nanostructure surfaces. Small 2009, 5: 2460–2466. 10.1002/smll.200900688View Article
- Wang MH, Hu JW, Li YJ, Yeung ES: Au nanoparticle monolayers: preparation, structural conversion and their surface-enhanced Raman scattering effects. Nanotechnology 2010, 21: 145608. 10.1088/0957-4484/21/14/145608View Article
- Huang J, Zhang LM, Chen B, Ji N, Chen FH, Zhang Y, Zhang ZJ: Nanocomposites of size-controlled gold nanoparticles and graphene oxide: formation and applications in SERS and catalysis. Nanoscale 2010, 2: 2733–2738. 10.1039/c0nr00473aView Article
- Rao YY, Chen QF, Dong J, Qian WP: Growth-sensitive 3D ordered gold nanoshells precursor composite arrays as SERS nanoprobes for assessing hydrogen peroxide scavenging activity. Analyst 2010, 136: 769–774.View Article
- El-Said WA, Kim TH, Kim H, Choi JW: Analysis of intracellular state based on controlled 3D nanostructures mediated surface enhanced Raman scattering. PLoS One 2011, 6: e15836. 10.1371/journal.pone.0015836View Article
- Zhang B, Xu P, Xie XM, Wei H, Li ZP, Mack NH, Han XJ, Xu HX, Wang HL: Acid-directed synthesis of SERS-active hierarchical assemblies of silver nanostructures. J Mater Chem 2010, 21: 2495–2501.View Article
- Huang P, Yang D, Zhang C, Lin J, He M, Bao L, Cui DX: Protein-directed one-pot synthesis of Ag microspheres with good biocompatibility and enhancement of radiation effects on gastric cancer cells. Nanoscale 2011, 3: 3623–3626. 10.1039/c1nr10586hView Article
- Yang DP, Chen SH, Huang P, Wang XS, Jiang WQ, Pandoli O, Cui DX: Bacteria-template synthesized silver microspheres with hollow and porous structures as excellent SERS substrate. Green Chem 2010, 12: 2038–2042. 10.1039/c0gc00431fView Article
- Yang H, Li D, He R, Guo Q, Wang K, Zhang XQ, Huang P, Cui DX: A novel quantum dots-based point of care test for syphilis. Nanoscale Res Lett 2010, 5: 875–881. 10.1007/s11671-010-9578-1View Article
- Weddemann A, Ennen I, Regtmeier A, Albon C, Wolff A, Eckstädt K, Mill N, Peter MKH, Mattay J, Plattner C: Review and outlook: from single nanoparticles to self-assembled monolayers and granular GMR sensors. Beilstein J Nanotechnol 2010, 1: 75–93.View Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.